Heteropoly Tungstate Supported on Metal Oxide Catalysts for Liquid Phase Oxidation of Benzyl Alcohol with Hydrogen Peroxide Han Xiaoxiang, ,a Kuang Yingying,a Xiong Chunhua,a Tang Xiujuan,b Chen Qing,a Wang Kuiwu,a Hung Chin-Te,c Liu Li-Lic and Liu Shang-
Article J. Braz. Chem. Soc. , Vol. 29, No. 1, 88-98, 2018.
Printed in Brazil - ©2018 Sociedade Brasileira de Química http://dx.doi.org/10.21577/0103-5053.20170117
Heteropoly Tungstate Supported on Metal Oxide Catalysts for Liquid Phase
Oxidation of Benzyl Alcohol with Hydrogen Peroxide
Han Xiaoxiang,* ,a
Kuang Yingying, a
Xiong Chunhua, a
Tang Xiujuan, b
Chen Qing, a
Wang Kuiwu, a
Hung Chin-Te, c
Liu Li-Li c and Liu Shang-Bin*
,c a Department of Applied Chemistry and b College of Environmental Science and Engineering,
Zhejiang Gongshang University, 310018 Hangzhou, Chinac
Institute of Atom and Molecular Sciences, Academic Sinica, 10617 Taipei, Taiwan
A series of metal oxide supported tungstophosphoric acid catalysts were prepared by
impregnation. The physicochemical and acidic properties of these materials were characterized
by a variety of different analytical and spectroscopic techniques, namely Fourier transform
infrared spectroscopy (FTIR), X-ray diffraction (XRD), Brunauer-Emmett-Teller (BET) method,
and nuclear magnetic resonance (NMR), and exploited as heterogeneous catalysts for selectiveoxidation of benzyl alcohol (BzOH) with hydrogen peroxide (H 2 O 2 ). Among them, 20 wt.% H 3 PW 12 O 40 /CeO 2 catalyst exhibited the best oxidative activity. Further process optimization by
response surface methodology (RSM) based on the Box-Behnken design model resulted in a
benzyl alcohol conversion of 95.2% and a benzaldehyde yield of 94.2% with 98.9% selectivity,
in good agreement with the experimental results. Kinetic studies based on an irreversible parallelreaction model led to an activation energy (E a ) of 44.73 kJ mol -1 .
Keywords: ceria, heteropolyacid, oxidation, reaction engineering, process optimizationIntroduction
Aldehydes and ketones, which are important chemical intermediates, play critical roles in chemical industries and have been extensively used in drugs, additives and spices industries. 1-4 These carbonyl compounds are normally produced by selective catalytic oxidation, which has been widely used in clean production of chemicals. 5-9 One of the major concerns for oxidation reaction is product selectivity, a challenge arising from the fact that most products are thermodynamically unstable. Typically, transition-metal salts or complexes, especially precious metals, are commonly used as homogeneous or heterogeneous catalysts for oxidation reactions. 10 However, excessive consumptions of these metal catalysts are not only cost-ineffective but also created a great number of heavy-metal wastes. Thus, the development of green, cheap, and efficient catalyst systems is a demanding task. In this context, the research and development (R&D) of eco-friendly catalysts such as polyoxometalates (POMs) catalysts have received considerable attention. Among them, heteropolyacids (HPAs) with Keggin-type structure, which possess unique features such as low volatility, non- corrosive, non-toxic, strong Brønsted acidic strength, and excellent redox properties, have been extensively studied and utilized as solid acid catalyst for heterogeneous reactions. 11-14 Nonetheless, owing to their high solubility in polar solvents, HPA-based catalyst systems are drawback by their difficulty in catalyst separation and recycling. As such, modified HPA catalysts, particularly those that may be easily prepared using a feasible support, open up a wide new possibilities to unravel the aforementioned problems. 15-18 As such, while metal or heteroatom substituted HPAs with an exotic variety of structures and compositions have been widely utilized in heterogeneous and/or homogeneous reactions, 19-21 it is highly desirable to support them on a porous solid substrate with unique catalytic and porous properties. The high surface area available for the supported HPA catalyst was found to promote diffusion of reactants/products and dispersion of active sites to warren high catalytic activity with improved product quality, reduced production costs as well as a prolonged catalyst life due to improved robustness, recovery, and recyclability. 22-26
In the present work, we aim at the preparation of ceria
Xiaoxiang et al.
89 Vol. 29, No. 1, 2018
HPW) catalysts by means of incipient wetness impregnation method. The physicochemical properties of these HPW/CeO 2 composites were characterized by a variety of different techniques, viz. Fourier transform infrared spectroscopy (FTIR), X-ray diffraction (XRD), Brunauer- Emmett-Teller (BET) method, and solid-state 31 P magic-angle spinning (MAS) nuclear magnetic resonance (NMR). The catalytic performances of these supported catalysts were assessed by oxidation of benzyl alcohol (BzOH) with hydrogen peroxide (H 2 O 2 ). The corresponding reaction process and product optimization were studied by response surface methodology (RSM) and a kinetic model was also established for the alcohol oxidation reaction under optimized conditions. The satisfying catalytic activity observed for the supported HPW/CeO 2 catalysts may be attributed to the unique redox properties and oxygen storage capacity (OSC) 27-30 as well as the desirable strong acidity and capability of activating oxidant during oxidation of alcohol. 31,32 By comparison, other POMs-based catalysts such as PMo 11 Co showed lower catalytic activity with only ca. 51% benzaldehyde yield during oxidation of BzOH with H 2 O 2 . 21 Experimental
Materials and catalyst preparation
Analytical grade ceria (CeO 2 ), titania (TiO 2 ), zirconia (ZrO 2 ), benzyl alcohol (C 6 H 5 CH 2 OH; BzOH), hydrogen peroxide (H 2 O 2 , 30%), tungstophosphoric acid (H 3 PW 12 O 40 ;
HPW), and other chemicals were purchased commercially and used without further purification unless otherwise specified.
All supported HPW/CeO 2 catalysts were synthesized using an incipient wetness impregnation method with varied HPW to total weight of HPW and CeO 2 ratios.
The supported catalyst samples so prepared are hereafter denoted as xHPW/CeO 2 , where x = 15-25 wt.%. For example, the 20HPW/CeO 2 catalyst was prepared by impregnating ca. 4.0 g of ceria support with a 3 mL aqueous solution of HPW (115.8 mmol L -1 ) for 12 h, followed by first drying overnight at 120 °C, then calcined at 250 °C in static air for 4 h. Similar procedures were used to prepare other supported catalysts.
FTIR measurements were performed at room temperature on a Bruker IFS28 spectrometer. Each spectrum was accumulated by 32 scans between the diffraction (XRD) studies were conducted on a Bruker
D8 ADVANCE diffractometer equipped with a Ni-filtered Cu K α radiation operated at 40 kV and 20 mA. The room temperature XRD patterns were recorded within a 2 θ angle range of 5-80° at a scanning rate of 10° min -1 . N 2 adsorption/desorption isotherm measurements were performed on a Quantachrome NOVA 1000e physisorption analyzer operating at −196 °C. The acid properties of various catalyst samples were characterized by means of a 31 P-TMPO MAS NMR approach, namely solid-state 31 P magic-angle spinning (MAS) NMR of adsorbed trimethylphosphine oxide (TMPO) probe molecule. 33-37 All 31 P spectra of adsorbed TMPO on various solid acid catalyst samples were recorded at a Larmor frequency of 202.46 MHz using a single-pulse sequence under the conditions: pulse-width ( π/6), 1.5 µs; recycle delay, 10.0 s; sample spinning rate, 12 kHz. The 31 P chemical shifts ( δ 31 P) were referred to that of 85% H 3 PO 4 aqueous solution. Detailed sample preparing procedures involved for acidity characterization using the 31 P-TMPO MAS NMR approach can be found elsewhere. 33,34,39
The catalytic activities of various catalysts were assessed by oxidation of benzyl alcohol (BzOH) with hydrogen peroxide (H 2 O 2 ). The reactions were conducted in a reactor consisting of a three-necked flask (100 mL) and a condenser. Typically, equal molar amount (0.05 M) of BzOH and H 2 O 2 were introduced to the catalyst in the reactor, the mixture was stirred at a desired reaction temperature for a given period of time. Upon completion of reaction, the reaction mixture was separated by extraction with ethyl acetate. A gas chromatography (GC; Agilent 7890B) analyzer equipped with a flame ionization detector (FID) and an HP-5 capillary column was used to analyze the compositions of reaction mixture in conjunction with authentic samples.
Experimental design and mathematical model
On the basis of single factor experiments, response surface methodology (RSM) study assisted by a Design- Expert 6.0.5 software (Stat-Ease, USA) was employed to optimize the reaction parameters of BzOH oxidation reaction over the 20HPW/CeO 2 catalyst, which was found to show best catalytic performance (vide infra). A three- level, four-variable Box-Behnken design (BBD) model was adopted to investigate the effects of four independent process variables, namely amount of catalyst (x 1 ),
(4) where k represents the pre-exponential factor, R is the gas constant, and T is the reaction temperature.
Range and level
Table 1. List of symbols for various experimental variables and corresponding coded levels and ranges adopted in the experimental design Variable Symbol
Heteropoly Tungstate Supported on Metal Oxide Catalysts for Liquid Phase Oxidation of Benzyl Alcohol J. Braz. Chem. Soc.
, which may be attributed to asymmetric stretching vibrations of P–O, terminal vibration of W=O, corner-sharing W–O b –W, and edge- sharing W–Oc–W bonds, respectively, are characteristic bands anticipated for the Keggin-type unit of the PW 12 O 40 3– (PW) polyanions. 39 Clearly, these characteristic peaks are absent in the FTIR spectrum observed for the pure
FTIR spectroscopy is employed to elucidate chemical compositions and local configurations of various catalyst samples. The FTIR spectra of CeO 2 , HPW and HPW/CeO 2 with varied HPW loadings are shown in Figure 1. Similar to the pristine HPW (Figure 1a), the supported HPW/CeO 2 catalysts showed multiple absorption bands between 4000 and 400 cm –1 (Figures 1c-1e). The broad overlapping absorption bands centering at ca. 3435 cm
- –1 may be ascribed to stretching vibrations of O–H. The signals at 1080, 983, 889, and 804 cm –1
Results and Discussion Characterization of catalysts
- –1 +1 Amount of catalyst / g
0.9 Alcohol/hydrogen peroxide / (mol mol -1 ) x 2 1:1 1:2 1:3 Reaction time / h x 3
(1) where x i and x j (i, j = 1-4) represents the coded levels of various independent variables, and β , β i , β ii , and β ij are regression coefficients representing the offset, linear, quadratic, and interactive terms of the variables, respectively.
All factors in the experiment were coded into three levels, namely −1, 0, and +1 as shown in Table 1. A total of 29 experimental sets, including 24 factorial points and 5 central points, were adopted for the experimental design. Accordingly, the predicted response (product yield; Y) may be expressed as:
amount of water (x 4 ), on primary product yield, that is, benzaldehyde (BzH).
5 Amount of water / mL x
(3) where denotes the modified rate constant. By measuring the k values at various temperatures, the activation energy (E a ) could be derived from the Arrhenius
(2) where C A and C B represents the concentration of BzOH and H 2 O 2 , respectively, k’ is the rate constant, and α and β denote the reaction order of BzOH and H 2 O 2 , respectively. By taking the natural log of both sides, the above equation may further be expressed as:
The kinetic parameters associated with conversion of BzOH were also monitored for the 20HPW/CeO 2 catalyst. By varying the reaction times and temperatures the reaction rate (r) for oxidation of BzOH with H 2 O 2 to BzH may be derived by the equation:
25 Figure 1. FTIR spectra of (a) the pristine HPW; (b) pure CeO 2 ;
CeO 2 support (Figure 1b). Moreover, the presence of weaker absorption bands at ca. 598 and 516 cm
- –1 may be attributed to symmetric vibrations of O–P–O and W–O–W, respectively. 33 Regardless of minor variations in intensities of characteristic bands responsible for the PW polyanions, their presence in all supported HPW/CeO 2 catalysts confirm that Keggin structure remains intact upon supporting varied
- – 3.15x 1<
- 0.19x 1
- – 2.34x 2<
- – 2.49x 2<
- 0.22x 3
- -1 41 Likewise, by varying the initial concentrations of H O (81.3 kJ mol ) and for the oxidation of furfuryl alcohol 2 2 2 (i.e., C ), an H O reaction order ( β) of 0.38 with R = 0.999 over heterogeneous nano zirconium chromate catalyst in B 2 2
- -1 42 was obtained, as seen in Figure 7. THF (76.7 kJ mol ). This indicates that the 20HPW/CeO 2 Moreover, by plotting the variations of BzOH catalyst is indeed a highly effective catalyst for oxidation concentration (i.e., C ) versus reaction time during of benzyl alcohol to benzaldehyde. A oxidation of BzOH over the 20HPW/CeO catalyst under 2 the optimized reaction conditions (namely, amount of Conclusions
- -1 catalyst = 0.84 g, BzOH/H O = 1:1.2 mol mol , reaction 2 2 time 4.4 h, and amount of water of 22.3 mL), the rate Composite catalysts synthesized by incorporating the constants at different reaction temperatures may be superacidic tungstophosphoric acid (HPW) on a ceria obtained, as shown in Figure 8a. Accordingly, based on (CeO ) support have been successfully prepared and 2 equation 4, the Arrhenius plot of ln k vs. 1/T in Figure 8b exploited for oxidation of benzyl alcohol (BzOH) with may be used to derive the activation energy (Ea) of the hydrogen peroxide (H O ). Among various composite -1 2 2 reaction, which is 44.7 kJ mol . Overall, the rate equation catalysts examined, the catalyst of 20HPW/CeO loaded 2 for oxidation of BzOH with H O over the 20HPW/CeO with 20 wt.% of HPW was found to exhibit satisfying 2 2 2 catalyst may readily be written as: catalytic activity with excellent BzOH conversion (94.0%)
- -1 2 2 catalyst, 22.22 g L .
- -1 2 2
Xiaoxiang et al.
91 Vol. 29, No. 1, 2018
amounts of HPW onto the CeO 2 support.
The crystalline structures of the pure CeO 2 , pristine HPW, and various supported HPW/CeO 2 composites with varied HPW loadings were examined by XRD, as shown in Figure 2. The CeO 2 support exhibited XRD profile with well-defined diffraction peaks at 2 θ angles of 28.5,
33.4, 46.6, 56.7, 58.0, 69.2, 76.2, and 78.9° (Figure 2a), corresponding to the crystalline lattice planes of (111), (200), (220), (311), (222), (400), (331), and (420), respectively. The above diffraction peaks observed for the as-prepared CeO 2 are in excellent agreement with the face center cubic
(fcc) phase structure of ceria (JCPDS Card No. 34-394), as expected. On the other hand, the XRD profile of pristine HPW showed characteristic diffraction pattern anticipated for the PW Keggin unit with main peaks at 10.3, 25.3, and 34.6 ° (Figure 2b). 26,39 However, these characteristic features were invisible in various supported xHPW/CeO 2 (x = 15, 20, and 25 wt.%) composite materials (Figures 2c-2e). Rather, the XRD profile observed for these supported catalysts were nearly identical with that observed for the as-prepared CeO 2
(Figure 2a). The above results suggested that the incorporated HPW are well-dispersed on the surfaces of the CeO 2 support. Together with the results obtained from FTIR spectroscopy, it is indicative that HPWs are successfully incorporated and homogeneously dispersed on the CeO 2 support.
Additional physisorption studies by N 2 adsorption/ desorption isotherm measurements have also been made (not shown). Accordingly, the pristine HPW and the pure CeO 2 samples gave rise to a BET surface area of 6.8 and
26.0 m 2 g -1 , respectively. However, a somewhat anticipated for the 15HPW/CeO 2 , 20HPW/CeO 2 , and 25HPW/CeO 2 catalysts, respectively. The consistent decrease in surface area with increasing HPW loading observed for the supported catalysts provides additional support to the above FTIR and XRD results to verify that the incorporated HPW was indeed nicely dispersed in the porous CeO 2 support. 40 The acid properties of various samples were monitored by solid-state 31 P MAS NMR using TMPO as probe molecule, which has been shown to be a powerful and reliable technique for acidity characterization. 34,35 Such 31 P-TMPO
NMR approach relies on the adsorption of a basic probe molecule TMPO onto the acid catalyst. Then the catalyst shows a desirable NMR-sensitive nuclei (i.e., 31 P) with a broad range chemical shift (denoted as δ 31 P). As a result, the probe molecule tends to interact with the available Brønsted acidic protons (H + ) site in the acid catalyst to form TMPOH + complexes with varied values of δ 31 P. It has been shown that detailed acid features such as acid types, concentration, distribution, and strength of acid catalysts may readily be determined by means of the 31 P-TMPO NMR approach. 34,35
This is made possible by the fact that a linear correlation between the observed δ 31 P and acidic strength may readily be inferred. 34-38 Moreover, the acid types and concentration may readily be determined by chemical shift assignment and spectral deconvolution of the observed 31 P spectrum. Accordingly, the 31 P NMR spectra of TMPO adsorbed on various catalysts are depicted in Figure 3. The spectrum observed for TMPO-adsorbed on pure CeO 2 revealed broad overlapping signals spanning between δ 31 P of ca. 35-55 ppm. The 31 P resonance centering at ca. 50 ppm should be due to physisorbed TMPO, whereas those centering at ca. 42 and 36 ppm may be attributed to bulk and mobile TMPO, respectively. As for TMPO adsorbed on the pristine TPA, broad resonances centering at three distinct regions with δ 31 P of –10 to –15, 55 to 75, and 80 to 95 ppm were observed
(Figure 3e), which may be ascribed due to PW Keggin unit, (TMPO) n H + adducts (n > 1.0), and TMPOH + complexes, respectively. 34,39 It is noteworthy that the catalyst showed superacidity which exceeds the threshold acidic strength for superacidity (86 ppm). 34-37,39 So the pristine HPW and supported HPW/CeO 2 possess superacidity. Unlike the pristine HPW, an additional peak at ca. 66 ppm was observed for all supported HPW/CeO 2 catalysts (Figures
3b-3d), indicating the presence of Lewis acidity arising from Ce metal centers. 34,35 Similar phenomenon was also found for HPW incorporated on other metal oxide supports such as ZrO 2 and TiO 2 , as illustrated in Figure 4. Moreover, it is indicative that the overall strength of acid sites (particularly those with δ 31 P > 80 ppm) of the supported HPW/CeO 2 catalysts follow the ascending trend:
Figure 2. XRD patterns of (a) CeO 2 ; (b) HPW; (c) 15HPW/CeO 2 ; (d) 20HPW/CeO 2 ; and (e) 25HPW/CeO 2 .
92 Heteropoly Tungstate Supported on Metal Oxide Catalysts for Liquid Phase Oxidation of Benzyl Alcohol J. Braz. Chem. Soc.
indicative that the incorporation of superacidic HPW onto the CeO support tends to provoke formation of Lewis 2 acidity. Together with the ultra-strong Brønsted acidity, a synergy effect due to Brønsted-Lewis acid sites may be inferred for the satisfying catalytic performance observed for the supported HPW/CeO catalysts during oxidation of 2 BzOH (vide infra).
Oxidation of benzyl alcohol to benzaldehyde
Table 2 summarizes the catalytic performances of various catalysts during oxidation of BzOH. The CeO 2 support, which possesses the weakest acidity, exhibited null activity for oxidation of BzOH. Upon incorporation of HPW onto CeO , a significant enhancement in catalytic activity 2 was observed. The 15HPW/CeO catalyst with HPW 2 31 loading of 15 wt.% showed satisfactory BzOH conversion
Figure 3. P NMR spectra of TMPO adsorbed on (a) CeO ; 2 and BzH product yield of 77.9 and 76.0%, respectively.
(b) 15HPW/CeO ; (c) 20HPW/CeO ; (d) 25HPW/CeO ; (e) pristine HPW. 2 2 2 Asterisks represent spinning sidebands.
Upon increasing the HPW loading to 20 wt.%, notable increases in both BzOH conversion (94.0%) and BzH yield (92.3%) with excellent selectivity (98.2%) were observed. However, further increase in HPW loading to 25 wt.% led to inferior performance, the BzOH conversion and BzH yield decreased to 93.2 and 88.4%, respectively. The effect of support on BzOH oxidation were also investigated, and the results obtained from 20 wt.% HPW on ZrO , TiO 2 2 and CeTiO supports are also depicted in Table 2. Even though CeTiO, TiO and ZrO were found to have a larger 2 2 2 -1 surface area (94, 53 and 33 m g , respectively) than CeO 2 -1 2
(8.1 m g ), it is obvious that the 20HPW/CeO catalyst 2 still outperformed its counterparts for oxidation of BzOH.
The satisfying catalytic performance observed for the
20HPW/CeO catalyst during oxidation of BzOH with H O 2 2 2 may be correlated to its acid properties, as evidenced by 31 results obtained from P MAS NMR of adsorbed TMPO (Figures 3 and 4) discussed above. Clearly, the presence 31 of excessive amount of ultra-strong acidity is detrimental
Figure 4. P NMR spectra of TMPO adsorbed on (a) 20HPW/ZrO ; 2
for oxidation of alcohol. As such, the satisfying catalytic
(b) 20HPW/CeO ; and (c) 20HPW/TiO . Asterisks represent spinning 2 2 sidebands. a Table 2. Comparisons of catalytic performances over various catalysts during oxidation of benzyl alcohol Catalyst BzOH conversion / % BzH selectivity / % BzH yield / % CeO nil nil nil 2
20HPW/ZrO 2 b
83.2 Reactions were performed under the conditions: BzOH/H O , 1:2 (mol mol ); amount of catalyst, 0.8 g; reaction time, 4 h; amount of water, 20 mL; 2 2
Xiaoxiang et al.
93 Vol. 29, No. 1, 2018
activity observed for the 20HPW/CeO 2 catalyst may be attributed to the presence of desirable amount of strong Brønsted and Lewis acid sites. In other word, it is due to a synergetic effect of Brønsted-Lewis acid sites. Since the
20HPW/CeO 2 catalyst exhibited the best catalytic performance for oxidation of BzOH to BzH, it was exploited for the subsequent process variable optimization and kinetic studies.
Effects of reaction parameters on oxidation of benzyl alcohol
The effects of experimental parameters such as amount of catalyst, reaction time, temperature, BzOH/H 2 O 2 molar ratio, and amount of water on catalytic performances during the oxidation reaction over the 20HPW/CeO 2 catalyst were studied. This is done by varying a target parameter while keeping the others fixed, as shown Figure 5. Both BzOH conversion and BzH yield increases with increasing catalyst amount (Figure 5a), reaching a plateau at ca. 0.8 g with a conversion and product yield of 94.0 and 92.3%, respectively. It is expected that more amount of catalyst in the reaction system warrants more available active moieties for catalyzing the reaction. Nevertheless, upon reacting a desirable amount of active moieties required for oxidation of BzOH, further increase in catalyst amount is redundant. Likewise, an optimal reaction time of 4 h (Figure 5b), reaction temperature of 110 °C (Figure 5c), BzOH/H 2 O 2 ratio of 1:2 (Figure 5d), and amount of water of 20 mL (Figure 5e) may also be inferred. It is anticipated that reaction carried out over extended period of time and elevated temperatures may provoke occurrence of undesirable side reactions. Moreover, a desirable excessive amounts of H 2 O 2 and water is favorable for driving the equilibrium towards formation of BzH, whilst an immense amount of H 2 O 2 tends to dilute the reaction system, which is unfavorable for BzH selectivity and yield. The presence
Figure 5. Effects of (a) amount of catalyst; (b) reaction time; (c) reaction temperature; (d) benzyl alcohol (BzOH) to hydrogen peroxide (H 2 O 2 ) molar ratio; and (e) amount of water on conversion () and benzaldehyde yield () during oxidation of BzOH with H 2 O 2 over the 20HPW/CeO 2 catalyst; (f) recyclability test. Unless otherwise specified, all reactions were performed under the typical conditions: amount of catalyst, 0.8 g; BzOH/H 2 O 2 , 1:1.2 (mol mol -1 ); reaction
1 −1 89.63 19 −1
17 −1 −1
1 −1 88.09 15 −1
13 −1 −1
1 −1 88.50 11 −1
88.30 23 −1
22 1 −1
21 −1 −1
9 −1 −1
Heteropoly Tungstate Supported on Metal Oxide Catalysts for Liquid Phase Oxidation of Benzyl Alcohol J. Braz. Chem. Soc.
A factorial analysis by analysis of variance (ANOVA) and response surface methodology (RSM) were utilized to investigate the interactive effects between experimental variables and to optimize process variables. Accordingly, the product yields (Y) predicted by multiple regression analysis may be predicted by means of a quadratic model: Y = 92.28 + 6.17x 1 + 2.13x 2 + 2.79x 3 + 1.99x 4 – 5.70x 1 2 –
RSM and ANOVA studies
1:2 (mol mol -1 ); reaction time, 4.0 h; amount of catalyst, 0.8 g; amount of water, 20.0 mL; and reaction temperature, 110 °C. As a result, a maximum BzOH conversion of 94.0% and a BzH selectivity and yield of 98.2 and 92.3%, respectively, may be achieved.
of water tends to form special droplets in the heterogeneous reaction system to favor adsorption and/or activation of oxidant during the oxidation reaction. Thus, it is conclusive that the best performance for efficient oxidation of BzOH with H 2 O 2 over the 20HPW/CeO 2 catalyst may be obtained under the optimal experimental conditions: BzOH/H 2 O 2 ,
Table 3. List of experimental design and response values obtained for oxidation of BzOH over the 20HPW/CeO 2 catalyst entry
Variable and level Yield / % x 1 x 2 x 3 x 4
1 −1 −1
1 −1 88.15 3 −1
5 −1 −1
1 −1 88.23 7 −1
3.41x 2 2 – 2.00x 3 2 – 2.58x 4 2 – 1.33x 1
Based on results obtained from RSM, the optimized reaction conditions for most effective oxidation of
x 4 (0.22) interactive terms in equation 5.
(Supplementary Information). The above observations are consistent with the ANOVA results depicted in Table 4 and coincide with the smaller coefficient observed for the x 1
(water amount) were more significant. Moreover, it is obvious that the most significant effect on BzH yield arose from interactions between amount of catalyst (x 1 ) and reaction time (x 3 ), as shown in Figures S1b and S2b
(BzOH/H 2 O 2 molar ratio) and x 3 (reaction time) and
Figures S1d and S1e revealed that correlations between
(5) where x 1 , x 2 , x 3 , and x 4 represent the coded values of the four process variables defined in Table 1, and the results are summarized in Table 3.
By fitting the experimental results with those predicted by RSM, the reliability of the fitting and validity of the proposed model in equation 5 may be assessed. As depicted in Table 4, a coefficient of determination (R 2 ) value of
0.9811 was achieved, revealing that only a minimal percentage (1.9%) of the fittings were unjustifiable by the model. Moreover, an F model value of 51.87 and a lack-of-fit of 3.78 were obtained, implying the lack-of-fit is not significant relative to the pure error. These results indicate that the proposed model was adequate and the fittings between the experimental and predicted results are highly reliable.
Based on the RSM results, the correlations between process variable pairs for oxidation of BzOH with H 2 O 2 over the 20HPW/CeO 2 catalyst may further be clarified by the contour plots and three-dimensional (3D) response surface plots shown in Figures S1 and S2 of the Supplementary Information, respectively. It was found that the correlations between catalyst loading (x 1 ) and BzOH/H 2 O 2 molar ratio (x 2 ), and that of reaction time (x 3 ) and water amount (x 4 ) on BzH yield were not significant, as evidenced by the nearly circular contour plots in Figures S1a and S1f. On
(0.19) and x 3
Xiaoxiang et al.
7.055.11 0.0403 b x 1 x 3
39.6328.71 0.0001 a x 1 x 4
0.150.11 0.7480 x 2 x 3
21.9015.87 0.0014 a x 2 x 4
24.7517.93 0.0008 a x 3 x 4
43.3331.39 < 0.0001 a x 1 x 2
0.190.14 0.7167 Residual
1.753.78 0.1061 NS Pure error
0.46Cor. total 1021.66
95 Vol. 29, No. 1, 2018
derived as the following: amount of catalyst (x 1 ) = 0.84 g, BzOH/H 2 O 2 ratio (x 2 ) = 1:1.19 mol mol -1 , reaction time
(x 3 ) = 4.43 h, and amount of water (x 4 ) = 22.31 mL, leading to a predicted BzH yield of 94.6%. These theoretical results are in excellent agreement with the experimental data. To further verify the validity of the predicted BzH yield, three parallel experiments were carried out independently over the 20HPW/CeO 2 catalyst using these predicted reaction variables. As a result, an experimental BzH yield of 94.2% was achieved (with BzOH conversion of 95.2% and BzH selectivity of 98.9%), in excellent agreement with the predicted yield (94.6%).
Catalyst recycling test
The durability and reusability of the 20HPW/CeO 2 catalyst for oxidation of BzOH with H 2 O 2 under the simplified process conditions, viz. amount of catalyst = 0.84 g, BzOH/H 2 O 2 molar ratio = 1:1.2 mol mol
, reaction time = 4.4 h, and amount of water = 22.3 mL, were further tested for six consecutive experimental runs. Note that, upon completion of each run, the catalyst was filtered and washed (by diethyl ether) and reused after drying under vacuum for 8 h at 70 °C. As shown reusability. The BzH yield and selectivity BzH decreased from ca. 94.2 and 98.9% of the initial cycle to ca. 92.1 and 96.8% of the 6 th cycle, respectively. Additional FTIR measurements also revealed that the structural integrity of the
20HPW/CeO 2 catalyst remained practically unchanged for the spent catalyst obtained after six consecutive runs (Figure S3; Supplementary Information). However, the yield of BzH was decreased largely to 85.4 and 79.3% for the 7 th and 8 th cycle, respectively. The decrease in catalytic activity observed during cyclic tests may be attributed to the loss of HPW during the regeneration treatment; as evidenced by elemental analyses using the inductively coupled plasma (ICP) technique (ICP-OES CID spectrometer, ICAP 6500; Thermo Scientific). It was found that the overall concentration of P atom decreased from 0.21 wt.% of the fresh catalyst to 0.13 wt.% of the regenerated spent catalyst obtained after eight running cycles. In spite of this drawback, the above results clearly indicate that the 20HPW/CeO 2 catalyst is indeed robust and durable for catalytic oxidation reaction, thus, render practical industrial applications.
The kinetic parameters involved during catalytic
Table 4. List of results obtained from ANOVA for BzH yield Source Sum of square DF Mean square F P > F Significance Model 1002.33
71.6051.87 < 0.0001 a x 1 456.21 1 456.21 330.52 < 0.0001 a x 2
54.7039.63 < 0.0001 a x 3
93.0767.43 < 0.0001 a x 4
47.6434.52 < 0.0001 a x 1 2 210.52 1 210.52 152.52 < 0.0001 a x 2 2
75.3554.59 < 0.0001 a x 3 2
25.8418.72 0.0007 a x 4 2
28 DF: degree of freedom; NS: non-significant; a highly significant; b significant.
96 Heteropoly Tungstate Supported on Metal Oxide Catalysts for Liquid Phase Oxidation of Benzyl Alcohol J. Braz. Chem. Soc.
also determined. As shown in Figure 6a, by monitoring (6)
BzOH conversion with varied initial concentrations (i.e., C ), the corresponding value of reaction rate (r) may A be obtained based on equation 2, while the reaction order It is noteworthy that the E value obtained for the present a of BzOH ( α) may be derived by equation 3, as shown in catalytic system for oxidation of BzOH is much lower
Figure 6b. As a result, an α value of 1.73 was obtained than that for oxidation of substituted phenethyl alcohols 2 with a satisfactory correlation coefficient (R ) of 0.996. over the N-chlorinated p-toluenesulfonamide (p-TSA) salt
Figure 6. (a) Variations of BzOH concentration (C ) versus reaction time; symbols for initial C values: 1.36 (), 1.23 (), 1.09 (), and 0.95 mol L ( );A A -1
(b) log-log plot of initial oxidation rate (r) vs. initial C . Reaction conditions: temperature, 110 °C; initial H O concentration, 2.73 mol L ; initial BzH-1 -1 A 2 2 concentration, 0 mol L ; amount of catalyst, 22.22 g L .
Figure 7. (a) Variations of H O concentration (C ) versus reaction time; symbols for initial C values: 2.72 (), 2.02 (), 1.31 (), and 0.95 mol L ( );2 2 B B -1
(b) log-log plot of initial oxidation rate vs. initial C . Reaction conditions: temperature, 110 °C; initial BzOH concentration, 1.36 mol L ; initial H OB 2 2
Vol. 29, No. 1, 2018 Xiaoxiang et al.
97 Figure 8. (a) Variations of BzOH concentration versus reaction time under different reaction temperatures: 95 (), 100 (), 105 (), and 110 °C ( ); -1 -1
(b) the corresponding Arrhenius plot; reaction conditions: initial BzOH concentration, 1.36 mol L ; initial H O concentration, 2.73 mol L ; amount of
and BzH yield (92.3%) and selectivity (98.2%). The 3. Choudhary, V. R.; Jha, R.; Jana, P.; Green Chem. 2007, 9, 267. satisfying catalytic activity observed for the composite 4. Friedrich, H. B.; Platinum Met. Rev. 1999, 43, 94. catalyst is attributed to the strong acidity and Brønsted-
5. Enache, D. I.; Edwards, J. K.; Landon, P.; Solsona-Espriu, B.;
Lewis acid synergy effect. Process optimization based on Carley, A. F.; Herzing, A. A.; Watanabe, M.; Kiely, C. J.; Knight, RSM rendered prediction of optimized reaction parameters, D. W.; Hutchings, G. J.; Science 2006, 311, 362. namely, amount of catalyst 0.84 g, BzOH/H O ratio
6. Cortés Corberán, V.; González-Pérez, M. E.; Martínez-
1:2 mol mol , reaction time 4.4 h, and amount of water González, S.; Gómez-Avilés, A.; Appl. Catal., A 2014, 474, 22.3 mL at a reaction temperature of 110 °C. Accordingly, the 211. value of BzOH conversion, BzH yield, and BzH selectivity
7. Liu, C. H.; Lin, C. Y.; Chen, J. L.; Lu, K. T.; Lee, J. F.; Chen, of 95.2, 94.2, and 98.9%, respectively, were derived, in good J. M.; J. Catal. 2017, 350, 21.
agreement with the experimental results. Such supported 8. Ahmad, J. U.; Räisänen, M. T.; Leskelä, M.; Repo, T.; Appl. HPW/CeO catalysts, which are cost-effective and may Catal., A 2009, 371, 17. 2 be easily prepared in mass quantity, also exhibit excellent
9. Sudarsanam, P.; Mallesham, B.; Naga Durgasri, D.; Reddy, B.
activity, durability, and recyclability, showing prospective M.; J. Ind. Eng. Chem. 2014, 20, 3115. applications for large-scale oxidation of alcohols.
10. Yu, X.; Huo, Y.; Yang, J.; Chang, S.; Ma, Y.; Huang, W.; Appl.
Surf. Sci. 2013 , 280, 450.
11. Kim, H. J.; Jeon, Y. K.; Park, J.; Shul, Y. G.; J. Mol. Catal. A: Chem. 2013, 378, 232.
Supplementary data associated with this article can
12. Farsani, M. R.; Jalilian, F.; Yadollahi, B.; Rudbari, H. A.; be found, in the online version, at http://jbcs.sbq.org.br Polyhedron 2014 , 76, 102.
as PDF file.
13. Tokarz-Sobieraj, R.; Grybos, R.; Filek, U.; Micek-Ilnicka, A.; Niemiec, P.; Kirpsza, A.; Witko, M.; Catal. Today 2015, 257, Acknowledgments 72.
14. Leng, Y.; Zhao, P.; Zhang, M.; Wang, J.; J. Mol. Catal. A: Chem.
The supports of this work by the Project of Science 2012, 358, 67. and Technology Department of Zhejiang Province (No.
15. Pamin, K.; Pro ńczuk, M.; Basąg, S.; Kubiak, W.; Sojka, Z.; 2016C31016), the Program for Zhejiang Leading Team Połtowicz, J.; Inorg. Chem. Commun. 2015, 59, 13.
of S & T Innovation (No. 2013TD07), and the Ministry of 16. Zhao, W.; Zhang, Y.; Ma, B.; Ding, Y.; Qiu, W.; Catal. Commun. Science and Technology, Taiwan (NSC 104-2113-M-001- 2010, 11, 527. 019) are gratefully acknowledged.
17. Farsani, M. R.; Yadollahi, B.; J. Mol. Catal. A: Chem. 2014, 392 , 8.
18. Choi, J. H.; Kang, T. H.; Song, J. H.; Bang, Y.; Song, I. K.; Catal. Commun. 2014 , 43, 155.
1. Xu, C.; Zhang, C.; Li, H.; Zhao, X.; Song, L.; Li, X.; Catal.
19. Dong, D. R.; Choi, J. H.; Park, S.; Song, I. K.; Appl. Catal., A Surv. Asia 2016 , 20, 13. 2011, 394, 201.
2. Du, Y. Y.; Wang, Q.; Liang, X.; He, Y. F.; Feng, J. T.; Li, D. Q.;
20. Wang, S. S.; Zhang, J.; Zhou, C. L.; Vo-Thanh, G.; Liu, Y.;
98 Heteropoly Tungstate Supported on Metal Oxide Catalysts for Liquid Phase Oxidation of Benzyl Alcohol J. Braz. Chem. Soc.
21. Pathan, S.; Patel, A.; Appl. Catal., A 2013, 459, 59.
34. Zheng, A.; Huang, S. J.; Liu, S. B.; Deng, F.; Phys. Chem. Chem.
22. Madhusudhan Rao, P.; Wolfson, A.; Kababya, S.; Vega, S.; Phys. 2011 , 13, 14889.
Landau, M. V.; J. Catal. 2005, 232, 210.
35. Zheng, A.; Li, S.; Liu, S. B.; Deng, F.; Acc. Chem. Res. 2016,
23. Chen, L. J.; Feng, T.; Wang, P. F.; Chen, Z. W.; Yana, R. Q.; 49 , 655.
Liao, B.; Xiang, Y. J.; Appl. Catal., A 2016, 523, 304.
36. Zheng, A.; Huang, S. J.; Chen, W. H.; Wu, P. H.; Zhang, H.;
24. Ghanbari-Siahkali, A.; Philippou, A.; Dwyer, J.; Anderson, M. Lee, H. K.; De Ménorval, L. C.; Deng, F.; Liu, S. B.; J. Phys.W.; Appl. Catal., A 2000, 192, 57. Chem. A 2008 , 112, 7349.
25. Izumi, Y.; Urabe, K.; Chem. Lett. 1981, 10, 663.
37. Zheng, A.; Zhang, H.; Lu, X.; Liu, S. B.; Deng, F.; J. Phys.
26. Hu, C.; He, Q.; Zhang, Y.; Liu, Y.; Zhang, Y.; Tang, T.; Zhang, Chem. B 2008 , 112, 4496.
J.; Wang, E.; Chem. Commun. 1996, 2, 121.
38. Essayem, N.; Gayraud, A. P. Y.; Vedrine, J. C.; Taarit, Y. B.; 27. Vlaic, G.; Di Monte, R.; Fornasiero, P.; Fonda, E.; Kaspar, J.; J. Catal. 2001, 197, 273. Graziani, M.; J. Catal. 1999, 182, 378.
39. Huang, S. J.; Yang, C. Y.; Zheng, A.; Feng, N.; Yu, N.; Wu, P.
28. Gokhan, E.; Demet, O.; Birgul, Z. K.; Catal. Commun. 2017, H.; Chang, Y. C.; Lin, Y. C.; Deng, F.; Liu, S. B.; Chem. Asian89 , 56.
J. 2011, 6, 137.
29. Reddy, B. M.; Khan, A.; Catal. Surv. Asia 2005, 9, 155.
40. Khder, A. E. R. S.; Hassan, H. M. A.; El-Shal, M. S.; Appl.
30. Narasimharao, K.; Ali, T. T.; Catal. Lett. 2013, 143, 1074. Catal., A 2012, 411-412, 77.
31. Zhang, H.; Xie, Y.; Sun, Z.; Tao, R.; Huang, C.; Zhao, Y.; Liu,
41. Ramachandra, H.; Rangappa, K. S.; Mahadevappa, D. S.;
Z.; Langmuir 2011, 27, 1152. MadeGowda, N. M.; Monatsh. Chem. 1996, 127, 241.
32. Abad, A.; Concepcion, P.; Corma, A.; Garcfa, H.; Angew. Chem., 42. Setareh, S.; Nooredin, G.; Monatsh. Chem. 2016, 147, 1531.
Int. Ed. 2005 , 44, 4066.
33. Ragupathi, C.; Judith Vijaya, J.; Narayanan, S.; Jesudoss, S. Submitted: January 25, 2017K.; John Kennedy, L.; Ceram. Int. 2015, 41, 2069. Published online: June 26, 2017